| ||Format||Pages||Price|| |
|3||$41.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$41.00||  ADD TO CART|
|Standard + Redline PDF Bundle||6||$49.20||  ADD TO CART|
This specification covers liquid membrane-forming compounds suitable for application to concrete surfaces to reduce the loss of water during the early-hardening period. White-pigmented membrane-forming compounds serve the additional purpose of reducing the temperature rise in concrete exposed to radiation from the sun. The membrane-forming compounds covered by this specification are suitable for use as curing media for fresh concrete, and may also be used for further curing of concrete after removal of forms or after initial moist curing. Liquid membrane-forming compound types 1 and 1-D shall be clear or translucent. Type 2 liquid membrane-forming compounds shall consist of finely-divided white pigment and vehicle, ready-mixed for immediate use as is. Liquid membrane-forming compounds, when tested, shall restrict the loss of water not more than the requirements prescribed. Type 2 liquid membrane-forming compounds, when tested, shall exhibit a daylight reflectance of not less than 60 %. Liquid membrane-forming compounds, when tested, shall dry to touch in not more than 4 h.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers liquid membrane-forming compounds suitable for application to concrete surfaces to reduce the loss of water during the early-hardening period. White-pigmented membrane-forming compounds serve the additional purpose of reducing the temperature rise in concrete exposed to radiation from the sun. The membrane-forming compounds covered by this specification are suitable for use as curing media for fresh concrete, and may also be used for further curing of concrete after removal of forms or after initial moist curing.
Note 1—This specification addresses only those properties listed in Sections 5 through 8. Membrane-forming compounds with special properties including better water retention, minimum solids content, resistance to ultraviolet radiation, acid and alkali resistance and non-interference with adhesives are described in Specification C1315.
Note 2—Solutions of silicate salts are chemically reactive in concrete rather than membrane-forming; therefore, they do not meet the intent of this specification.
1.2 The values stated in SI units are to be regarded as the standard. The values given in parentheses are provided for informational purposes only.
1.3 The following precautionary caveat pertains only to the test methods portion, Section 10, of this specification: This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
1.4 The text of this standard references notes and footnotes which provide explanatory material. These notes and footnotes shall not be considered as requirements of the standard.
1.5 This is a performance specification. The allowable composition of products covered by this specification is limited by various local, regional, and national regulations. Issues related to air quality (solvent emission), worker exposure, and other hazards are not addressed here. It is the responsibility of the producers and users of these materials to comply with pertinent regulations.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C156 Test Method for Water Loss [from a Mortar Specimen] Through Liquid Membrane-Forming Curing Compounds for Concrete
C1315 Specification for Liquid Membrane-Forming Compounds Having Special Properties for Curing and Sealing Concrete
D869 Test Method for Evaluating Degree of Settling of Paint
D883 Terminology Relating to Plastics
D1309 Test Method for Settling Properties of Traffic Paints During Storage
D2369 Test Method for Volatile Content of Coatings
E1347 Test Method for Color and Color-Difference Measurement by Tristimulus Colorimetry
ICS Number Code 91.100.30 (Concrete and concrete products)
UNSPSC Code 30111500(Concrete and mortars)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C309-11, Standard Specification for Liquid Membrane-Forming Compounds for Curing Concrete, ASTM International, West Conshohocken, PA, 2011, www.astm.orgBack to Top